Shape and deposition angle control of silver ﬁlm-over-nanosphere SERS substrates
Nasim Seyedpour Esmaeilzad1,∗ , Özge Demirtaş1 , Ahmet Kemal Demir2 and Alpan Bek1,3
1Micro and Nanotechnology Program, Middle East Technical University, 06800 Ankara, Turkey
2Department of Physics, Bilkent University, 06800 Ankara, Turkey
3Department of Physics, Middle East Technical University, 06800 Ankara, Turkey E-mail:email@example.com
Received 8 July 2021, revised 3 September 2021 Accepted for publication 16 September 2021 Published 6 October 2021
Thin metallicﬁlms on dielectric nanospheres are demonstrated to have a high potential for the fabrication of cost-effective SERS substrates. In addition to the morphological advantages that nanospheres offer for attaining a high density of hot spots, possessing shape adjustability by uncomplicated thermal treatment makes them an attractive platform for tuneable SERS substrates. Furthermore, when combined with the oblique angle metal deposition technique, adjustable gaps at a high density and adjustable shape of metalﬁlms, such as Ag ﬁlms, can be achieved on nanospheres. Applying small changes in deposition angle can provide means for ﬁne adjustment of the Raman enhancement factor (EF), resulting in EF up to 108measured using crystal violet dye molecule as a Raman analyte. This practice paves the way for the fabrication of high EF SERS substrates at a reasonable cost using a monolayer of self-organized nanosphere patterns. An ultra-thin Agﬁlm coated at 5° tilt is shown to be an excellent substitute for a ﬁlm deposited at 0° with double the thickness. There is a strong agreement between the experimental results andﬁnite-elements-method-based Maxwell simulations exhibiting expected ﬁeld enhancements up to 109at a tilt angle of 5°.
Supplementary material for this article is availableonline
Keywords: nanospheres, enhanced Raman spectroscopy, oblique angle deposition, shape control (Some ﬁgures may appear in colour only in the online journal)
Raman spectroscopy is a highly sensitive optical character- ization technique, which identiﬁes the chemical components of a material employing inelastic scattering of incident electro- magnetic radiation due to vibrations of chemical groups con- stituting the material. The Raman scattering, however, is a nonresonant low probability process as compared to resonant scattering processes such as elastic (Rayleigh) scattering or ﬂuorescence. Inherently low signal/noise in Raman measure- ments leading to relatively high molecular detection limits have urged scientists to employ several signal ampliﬁcations schemes such as surface-enhanced Raman spectroscopy
(SERS) [1–4], resonant Raman scattering [5,6], and coherent anti-Stokes Raman scattering(CARS) [7,8]. Resonant Raman scattering and CARS techniques involve highly speciﬁc light sources such as tuneable lasers and a high level of experimental complexity; therefore, SERS stands out as the most widely utilized signal ampliﬁcation technique in Raman spectroscopy.
SERS has two main origins: chemical and physical enhance- ment [9–12]. Chemical processes such as charge transfer can lead to 103fold enhancement, where physical processes can lead to 109–1012fold enhancement[14,15] of the Raman signal. The physical enhancement in SERS is based on enhanced localized electromagnetic ﬁelds, which can be achieved by surface plasmon resonances (SPR) of metal nanostructures [1–4, 16]. Commonly, SERS enhancement factors (EFs) are found to be highest in nanostructured noble
Nanotechnology 32(2021) 505709 (8pp) https://doi.org/10.1088/1361-6528/ac2765
∗ Author to whom any correspondence should be addressed.
0957-4484/21/505709+08$33.00 1 © 2021 IOP Publishing Ltd Printed in the UK
metal ﬁlm surfaces  or noble metal nano/microparticles that sustain strong ﬁeld localization due to the presence of localized SPR(LSPR) and a high density of so-called hot spots [18,19]. Based on electromagnetic simulations such as Max- well’s equations solvers and experimental results, it can be concluded that EFs in SERS can be considerably improved if the LSPR band centre is close to the excitation wavelength [20–23]. Due to its straightforward integration into standard Raman spectroscopy systems, as simple as the replacement of standard substrates with SERS substrates, SERS has found its place in a wide variety of applications in chemical and biolo- gical sensing[24–27].
SERS substrates based on metallic structures can be fabricated using a wide variety of approaches, such as nanoparticle self-assembly, e-beam lithography , and nanosphere lithography (NSL) . Among these methods, NSL has attracted considerable interest since it is a low-cost, robust, and reproducible method used for the fabrication of large area, ordered metal nanostructures. In NSL, hexagonally close-packed(hcp) polystyrene (PS) or silica nanosphere (NS) arrays are used as 2D masks to deposit metal nanostructures using thermal evaporation followed by removal of colloidal masks to form ordered triangular metallic nanostructures [31–34]. Another effective approach to achieve SERS sub- strates is keeping the colloidal NSL mask after metal eva- poration. This is because the metalﬁlm on the nanospheres has a considerable roughness, which can improve the Raman signal substantially[35–41]. This method, also referred to as a metalﬁlm over nanospheres (FONs) or metal-capped nano- spheres, can be employed for SERS detection of anthrax, glucose, biotin, and DNA[42–47].
The main privilege of the NSL method is that the tun- ability of the LSPR wavelength to the exciton wavelength is feasible as the plasmonic characteristics can be easily tuned by changing the size of nanospheres and thickness of the evaporated metalﬁlm . There are several reports in lit- erature targeting improvement or tunability of NSL based SERS substrate design. In one such work, it is targeted to increase the tunability of FON structures by deposition of Ag FONs on PDMS . In another work, a proposed method
for improvement is to coat the NSL mask with a bilayer of Ag and Au at the same thickness and determine optimized values for strong SERS signals . In another study, the LSPR wavelength is tuned by using silica nanospheres with different diameters, but the thickness of Ag is constant . Despite the practicality of such methods, it is beneﬁcial to employ a technique that does not require different nanosphere dia- meters, and the LSPR wavelength shift can be achieved by Ag ﬁlms over the NSL mask (AgFONs) with shape mod- iﬁcation. In that respect, the oblique angle deposition method can pave the way to tune the LSPR wavelength by changing the vapor incident angle relative to the surface normal of the substrate. The Raman enhancement in such a structure is mainly due to the Ag ﬁlm on the nanosphere rather than the underlying triangular islands.
Our study shows that a novel approach that combines two simple strategies can lead to attaining higher EF in SERS.
Firstly, a single-size NSL mask is shape-modiﬁed using a simple and swift annealing-based technique to enhance elec- tric ﬁeld concentration, consequently leading to high SERS EFs . Secondly, oblique deposition of Ag ﬁlms on a shape-modiﬁed NSL mask, albeit at low tilt-angles, is employed forﬁne tuning the EFs. The idea of oblique angle deposition was previously used in using larger θ resulting in not only a smaller Ag coating area but also in anisotropic thickness, which is not always desirable. Therefore, in our work, a custom-built thermal evaporation chamber is utilized to enable depositions at smaller angles, which enable ﬁne adjustment of the LSPR wavelength.
Crystal violet(CV), one of the most popular tracer dyes, was opted as the analyte to check the SERS response. Then, a relative EF is calculated by comparing the SERS spectra of CV acquired on AgFON substrates with Ag coated and bare Si wafers.
The SERS activity is measured using population statis- tics, which demonstrates that shape controlled AgFON monolayer substrates are very promising for a trace amount of molecule detection offering EFs up to 108, which is in good agreement with the ﬁnite element method (FEM) based Maxwell solver simulations.
2. Experimental methods 2.1. Preparation of AgFON arrays
2 cm×2 cm pieces of single-side polished silicon (Si) wafers are ultrasonically cleaned using acetone, isopropanol, and deionized water in sequence. A mild oxygen plasma treatment is carried out to make the surface of silicon samples hydro- philic. The solution of colloidal NSs, dispersed in water and functionalized with a hydroxyl group, was spin-coated on the Si samples. PS NSs self-organize in a hcp structure during the natural evaporation at room temperature, which is commonly used as the NSL mask in literature. Fabrication of NSL with this method yields about 5% of multilayers close to the sample edges and an overwhelming 95% of the central regions of the samples end in a monolayer structure. A low
Figure 1.(a) Shape-modiﬁed hcp PS NSs on Si wafer, (b) Oblique angle deposition of an Agﬁlm over PS NSs, (c) Top view of the Ag coated nanospheres depicting theﬁeld enhancement, (d) A simpliﬁed sketch of a nanosphere with the CV molecules(note: a continuous molecular coating is assumed in calculations).
magniﬁcation SEM image is provided in the supplementary ﬁle (ﬁgure S1 available online atstacks.iop.org/NANO/32/505709/
mmedia) displaying the quality of large-area monolayers.
Subsequent thermal treatment of the NSL mask improves the adhesion of PS NSs to the Si surface. We have experi- enced that the NSs tend not to stayﬁxed on the surface of Si during coating of the dye molecules from aqueous solution unless this thermal treatment is employed, which is done at 110°C for 20 min .
The diameters of PS NS employed for SERS substrates are 350 nm. Ag ﬁlms are deposited at two different thick- nesses of 10 nm and 20 nm on a monolayer PS NS based NSL mask using a custom-built thermal evaporation deposition system at incidence angles ofθ=0°, 5°, 10°, 15°.
The fabrication steps are shown inﬁgure 1. First, a PS NS-based NSL mask is fabricated and annealed at 110°C for 20 min on a hot plate(ﬁgure1(a)). Next, thermal evaporation- based oblique angle Ag deposition is performed on the NSL mask, and fabrication of the AgFON array is ﬁnalized, as shown in ﬁgure 1(b). CV molecules are spin-coated on an AgFON array from an aqueous solution at 10−4 mol l−1 concentration. Figure 1(c) shows the ﬁeld enhancement of nanospheres.
2.2. Sample characterization
The SEM images in ﬁgure 2 display the AgFON array structure viewed from different angles and at different mag- niﬁcations. Figure 2(a) shows a top-view image of the AgFON array in which a uniform self-organized hcp con- ﬁguration of 350 nm size NSs is clearly visible. Figure 2(b) shows a side-view image of NSs after annealing for 20 min at a temperature of 110°C. Figure2(c) displays the shadowing effect due to tilted evaporation.
2.3. SERS measurements
A 10−4 M CV solution was used as an analyte for SERS measurements. AgFONs were spin-coated with CV
molecules. The SERS signals were excited by using a linearly polarized continuous wave (CW) 532 nm wavelength laser source(Coherent Verdi) multimode (MM) ﬁber coupled to a modiﬁed upright microscope (Nikon Eclipse LV100) equip- ped with a 100X/0.90 NA objective. The excitation power is adjusted to 1.8 mW on the sample surface over a 17μm diameter round illumination spot. The incident polarization of the originally linearly polarized excitation laser is scrambled due to MMﬁber delivery. The Raman signal was collected in epi-conﬁguration by the same objective lens and coupled into another multimode ﬁber through a suitable dichroic mirror (Semrock) and a notch ﬁlter (Semrock). The Raman signals were analyzed by a f/9.8, 750 mm spectrometer (Andor Shamrock SR750) with 150 l mm−1grating and an EMCCD camera (Andor Newton). The detailed explanation and setup sketch is provided inﬁgure S2 in the supplementary ﬁle.
COMSOL Multiphysics was employed to carry out FEM- based Maxwell simulations. A three-dimensional model of the AgFON was designed based on SEM images using COMSOL Multiphysics’s CAD and Autodesk Meshmixer. The simula- tions were conducted to calculate the ﬁeld enhancement of AgFON at different Ag deposition angle(θ) values from 0° to 15° (ﬁgure4). The SEM images show that the Ag patch on each nanosphere is smaller than a half-circle. A linearly polarized CW plane wave at 532 nm wavelength is used in the simulations. The shape and coverage of the AgFON are speciﬁed considering the θ and the relative orientation of the NS monolayer domain with respect to polarization direction (j) of light. It is important to simulate different incidence polarization angles to ensure that the results are not speciﬁc to a single chosen conﬁguration and the results adequately represent the experimental conditions. The dielectric function of Ag was taken from Johnson and Christy . Further explanation regarding the simulation is provided in supple- mentary information along with ﬁgures S3 and S4. Figure3 depicts the oblique deposition angles of θ of 0°, 5°, 10°and 15° with respect to the substrate as a sketch and simulation model(in grayscale).
The evaporation angle has a vital role to play as it can ﬁnely adjust the LSPR wavelength of AgFONs . The optical response of AgFONs is dependent on Ag nanos- tructures and Ag ﬁlm on NSs for small θ. The larger the deposition angle becomes, the smaller the intersphere gaps become due to the shadowing effect. There is a criticalθcwith no nano triangles (around 55°) . As we target SERS due to AgFONs and not the triangular Ag nanostructures, we have carried out our experiments and simulations at smaller θ to study ﬁne tuning. The simulation results of the maximum Raman EF as a function of polarization angle for deposition angleθ of 0°, 5°, 10°, and 15° are shown in ﬁgure4. In the Raman EF calculations, we employ the well-accepted approximation of EF=Eloc4 E
/ where Elocand E0are the local and the incident ﬁeld magnitudes, respectively. It is found that the Raman EF is maximized for θ=5° for all incidence polarizations.
Figure 2.SEM images of(a) as-deposited hcp PS NSs with 350 nm size in top view,(b) 20 min 110 °C annealed PS NSs in side-view, (c) 5° tilt Ag deposited annealed PS NSs showing the shadowing effect.
When θ>5°, the EF has a considerable drop. The connection between EF andθ can be explained by the var- iation in the shape and coverage of Agﬁlm, which takes place during oblique angle deposition. Dark ﬁeld scattering spectroscopy measurements also display great agreement with FEM results, which can be seen in supplementary information ﬁgure S5.
3. Results and discussion 3.1. EF calculation
A unique deﬁnition of the EF is impossible due to experiment dependent situations such as single molecules, multiple molecules, experimental limitations, spatial distribution, orientations of the probe on the surface, etc. In fact, EF can strongly depend on the exact SERS conditions: substrate, analyte, excitation wavelength, etc. Kamaliya et al pre- dicted SERS EF from the hybrid gold-nanocone/graphene/
gold-nanohole tri-layers system via FDTD simulations. As nanocones are randomly spaced over the surface, three pos- sible geometrical conﬁgurations are considered for the FDTD simulations: nanocone is-(i) far from the nanohole, (ii) at the center of the nanohole, and(iii) at the edge of the nanohole.
For the conﬁguration where the nanocone is at the edge of the nanohole, the maximum EF of 1.05×109 for yz-plane is achieved with 600 nm wavelength excitation . Electro- magnetic SERS EFs at hot spots are predicted to be on the
order of ∼1010–1011, for example, at a junction between metallic particles . Because the single-molecule EF is the SERS enhancement on a given particular molecule at a speciﬁc point, it requires the exact deﬁnition of the SERS substrate geometry and the exact position and orientation of the probe on it . Etchegoin et al performed single-molecule SERS detection of a nonresonant molecule, adenine, using an iso- topically substituted adenine (N-adenine) as bianalyte SERS partners. They obtained maximum single-molecule EFs in the range of 7×1010–1×1011 for adenine and N-adenine, respectively. However, the average SERS EF is calculated by averaging the signals expected for molecules randomly adsorbed over all possible positions on the metallic surface.
Average SERS EFs are ∼101–103 for non-optimized condi- tions, ∼105–106 for ‘standard’ substrates, and ∼107–108 for very good SERS substrates. Because the maximum single- molecule EF only applies to one or a few localized regions of the surface, the average EFs are typically several orders of magnitude smaller. In addition, the average SERS EF is larger for more pointy structures, which increases with an increasing aspect ratio.
In normal Raman spectroscopy(NRS) inside liquid samples, the three-dimensional Raman probe volume can be determined by considering a prolate spheroid focal volume, which in our case have dimensions of rx=8.5 μm, ry=8.5 μm and rz(depth
Figure 3.Sketch of the oblique deposition angleθ and the corresponding SERS structures.
Figure 4.(a) Raman EF calculated using FEM simulations of AgFONs deposited at variousθ as a function of incident polarization angle.(b) Raman EFs belonging to 20 and 10 nm Ag coatings at 0°
and 5° of incidence.
of focus)=17 μm, yielding Vprobe=(4π/3)×8.5 μm
× 8.5 μm × 17 μm=5144.88 μm3=5.14×10−12l of probe volume. For our 10−4M solution, the total number of molecules (NNRS=CNRS X Vprobe) in the measurement volume can be found as NNRS=10−4 mol l−1×6.02×1023 molecules/mol×5.14×10−12 l=3.09×108 molecules.
After baseline correction, INRS is calculated through the area under the peak (1370 cm−1) with a width between 1350 and 1386 cm−1and is found as 322 cts s−1. Figure S6. in the sup- plementaryﬁle shows the SERS spectra together with the Raman spectrum of CV drop used for EF calculations. The Raman spectrum dominates theﬂuorescence of the CV molecule in the region of interest. In the estimation of the EFs, we considered a continuous molecular coating that extends to around 2 nm from the surface of the metalﬁlm while calculating the total number of CV molecules in the SERS measurements. In order not to overestimate the SERS EF, the number of molecules was mul- tiplied further by a factor of 2 in order to ensure that the experimentally determined values approximate the minimum EFs exhibited by the substrates. Any discontinuous coating effects would mean higher actual EFs than the estimated ones.
The molecules in the nearﬁeld extend to around 2 nm from the surface of the metal ﬁlm, resulting in a probe volume of Vprobe=2 nm×227×106 nm2×2=9.08×10−16 l. The number of molecules in the near ﬁeld was multiplied by 2 in order not to overestimate the EF. Therefore, the total number of CV molecules in the SERS measurement can be calculated as NSERS=10−4mol l−1×6.02×1023molecules/mol×9.08×
10−16 l=5.46×104molecules. The EF for surface averaged structures are calculated with the measured INRS and ISERS values as described above. Figure 5 shows the experimentally determined EFs where statistics of SERS measurements cover spectra acquired from 10 different random spots on each substrate prepared at different θ and Ag coating thicknesses before and after annealing of PS NSs. Peripheral regions of the samples are avoided to ensure the uniform monolayer structure of the NSL.
Statistics show that maximum EF is obtained from 10 nm Ag coating withθ = 5° on annealed PS NSs, which is con- sistent with the simulation results. It is observed that the variation of EF versus tilting angle is expected from simula- tions to take place more pronounced when compared to experimental results. The difference can be attributed to the following reasons. Firstly, perfect spherical geometry is used in simulations. The sharpness of edges between gaps of spheres can cause very strongﬁeld intensities in simulations.
However, in reality, the gaps exist between edges with edges ofﬁnite curvature, which have a limiting factor in achievable gap plasmon hotspotﬁeld intensity. A feature, which is most pronounced, especially in Ag, is due to its tendency for dewetting the underlying surface. Furthermore, there are collective effects in this study, and it is impossible to consider all the factors in simulations. For instance, grain boundaries and dislocations between the arrays of nanospheres, which are inevitable, are not considered in simulation results. Disloca- tions partially originate from theﬁnite size distribution of NS.
Besides, evaporation begins in different locations and even- tually uniﬁes, which causes multi-domains. Despite our extensive optimizations, about 5% of the total area is coated as bilayers or multilayers. As described before, despite our efforts to avoid them, their presence cannot be completely excluded. Also, our focus here is shape and angle control, which is done using universal measurements. Since mea- surements are performed at large-area illumination spots from ten different locations, our results correspond to the average Raman EF rather than the maximum achievable values. The simulations, however, highlight the maximum achievable Raman EFs. In addition, experimental EF is inﬂuenced by many different factors, including ﬁlm roughness, contribu- tions of propagating SPPs, propagating and localized gap plasmons, singular hotspots, etc. Overall effects of these factors contribute to the experimental results. It is true that in some cases, surface roughness alone can create hotspots. Yet sometimes, true nanometer-scale roughness can act as a deterrent for strong propagating SPPs due to the considerable amount of scattering they cause. In the case when the surface roughness is at a tiny length scale to produce hotspots, it can still lead to SPP damping. No additional roughness than what the nanospheres produce is considered in our simulations. It is expected that the EF factors in simulations are higher than the experimental results. They should be used in order to expect a theoretical trend of the dependence of the EFs to the control variables of the experiment. It is evident that with increasing the deposition angle, the shadowing effect causes reduction of the Ag coating area and increase of the Ag ﬁlm thickness variation.
Figure5shows that heat treatment-based shape control of PS NSs is a simple yet effective way to achieve homogeneous SERS substrates, as shown in the reduction of the population range in the box chart. Box charts show that not only does AgFON with 10 nm of thickness result in more homogenous SERS substrates but also enables signiﬁcant material cost reduction. This is because by applying simple annealing- based shape control and oblique angle Ag deposition, we can achieve EFs even better than that of the AgFON with 20 nm
Figure 5.Box charts displaying the population statistics of SERS EFs of(a) 10 nm and (b) 20 nm Ag coated PS NSs before (dotted lines) and after (solid lines) annealing with θ values of 0°, 5°, 10°
thickness coated at a normal deposition angle. So, it can be said that at least half the amount of Ag material can be saved using this method. It is also evident from ﬁgure5 that at a thickness of 20 nm, the shape control, and tilt angle do not yield statistically signiﬁcant changes in the EF. So, it can be said that these tuning parameters are most effective in achieving high EF SERS substrates with ultra-thin Ag layers.
It should be noted that AgFON overlaps at borders of the adjacent nanospheres, i.e. the edges of AgFON touch rather than leaving small gaps between nanospheres. It is expected that as the angle of deposition inclines, it is more likely for nanogaps between the nanospheres to emerge(such as at 5° of deposition angle). However, since the ﬁeld strength decreases with increasing gap width, it is also expected for the ﬁeld strength to decrease with a further inclination of the deposi- tion angle(such as at 10o of deposition angle and above). In conclusion, we expect to observe an optimal angle of deposition which would generate maximum ﬁeld enhance- ment. Assuming the gap effect to be the dominant mechanism for the EF, the coating material can be minimized to a thickness that is sufﬁcient to coat the nanosphere surface in a well-deﬁned fashion to generate gaps in a controllable fash- ion. One can see that a similar gap effect also occurs for 20 nm thickness, yet the order of magnitude of EFs for 10 nm and 20 nm are the same for 5° of deposition angle. So, one can save deposition material for the extra 10 nm of thickness.
For a clear understanding of the effect, the corresponding averaged SERS spectra are shown inﬁgure 6(a). It is evident that at the same Ag coating thickness of 10 nm, the Raman intensity can be enhanced around 103times on NSs with respect toﬂat Ag ﬁlm on Si. Moreover, a shape adjustment of the NSs followed by an oblique angle Ag evaporation at θ=5° can further improve the Raman signal substantially. Figure 6(b) clearly illustrates that with shape adjustment and oblique angle deposition, the necessary amount and hence the cost of Ag material can be cut by half. It should be noted that the consumed amount of evaporation material can easily be 3–4 orders of magnitude larger than the actual coated amount in thermal evaporators(depending on the source-sample distance).
In this study, annealing-based nanosphere shape adjustment and oblique angle deposition of Agﬁlm have been utilized as a method to fabricate SERS substrates at a low-cost. The small variation in deposition angle enablesﬁne tuning of the Raman enhancement factors of the AgFON structure. Raman enhancement factors as high as 108are achieved utilizing this technique from crystal violet dye molecule. This method enables cost-effective fabrication of SERS substrates with ultra-thin Ag ﬁlms deposited at 5° tilt can replace SERS substrates fabricated by deposition of Agﬁlms with double thickness in normal deposition angle. FEM simulations show excellent agreement with the experimental results and demonstrate expectedﬁeld enhancements up to 109at a tilt angle of 5°. This low-cost, high-performance SERS platform can be combined with further novel advances in theﬁeld .
This work was supported by The Scientiﬁc and Technological Research Council of Turkey (TÜBİTAK) under grant nr 119F101. ÖD acknowledges The Scientiﬁc and Technologi- cal Research Council of Turkey(TÜBİTAK) 2211-C program and Turkish Council of Higher Education YÖK 100/2000 program for the scholarships. We thank Ahmet Oral for giving access to the Raman spectrometer and the microscope.
Data availability statement
All data that support the ﬁndings of this study are included within the article (and any supplementary ﬁles).
Nasim Seyedpour Esmaeilzad https://orcid.org/0000- 0001-6551-0296
Özge Demirtaş https://orcid.org/0000-0002-1417-6491
Figure 6.SERS spectra of 10−4M CV spin-coated on(a) 10 nm Ag on non-annealed PS NSs(dotted blue line), annealed PS NSs with θ=5° (solid green line), and 10 nm Ag coating on Si (solid red line), (b) 10 nm Ag on annealed PS NSs with θ=5° (solid green line) and 20 nm Ag on non-annealed PS NSs without tilting (dotted blue line).
Ahmet Kemal Demir https://orcid.org/0000-0002- 3251-9793
Alpan Bek https://orcid.org/0000-0002-0190-7945
 Dobson P J 2014 Introduction to metal-nanoparticle plasmonics, by Matthew Pelton and Garnett W. Bryant Contemp. Phys.55 352–3
 Otto A 1983 Surface enhanced Raman scattering a otto Vaccum33 797–802
 Lin W C, Huang S H, Chen C L, Chen C C., Tsai D P and Chiang H P 2010 Controlling SERS intensity by tuning the size and height of a silver nanoparticle array Appl. Phys. A 101 185–9
 Pérez-Mayen L, Oliva J, Torres-Castro A and De La Rosa E 2015 SERS substrates fabricated with star-like gold nanoparticles for zeptomole detection of analytes Nanoscale 7 10249–58
 Calleja J M and Cardona M 1977 Resonant Raman scattering in ZnO Phys. Rev. B16 3753–61
 Renucci J B, Tyte R N and Cardona M 1975 Resonant Raman scattering in silicon Phys. Rev. B11 3885–95
 Potma E O, Evans C L and Xie X S 2006 Heterodyne coherent anti-stokes Raman scattering(CARS) imaging Opt. Lett. 31 241–3
 Day J P R, Domke K F, Rago G, Kano H, Hamaguchi H O, Vartiainen E M and Bonn M 2011 Quantitative coherent anti-stokes raman scattering(CARS) microscopy J. Phys.
Chem. B115 7713–25
 Valley N, Greeneltch N, Van Duyne R P and Schatz G C 2013 A look at the origin and magnitude of the chemical contribution to the enhancement mechanism of surface- enhanced Raman spectroscopy(SERS): theory and experiment J. Phys. Chem. Lett.4 2599–604
 Xia L, Chen M, Zhao X, Zhang Z, Xia J, Xu H and Sun M 2014 Visualized method of chemical enhancement mechanism on SERS and TERS J. Raman Spectrosc.45 533–40
 Yue W, Wang Z, Whittaker J, Lopez-Royo F, Yang Y and Zayats A V 2017 Ampliﬁcation of surface-enhanced Raman scattering due to substrate-mediated localized surface plasmons in gold nanodimers J. Mater. Chem. C5 4075–84  Stoerzinger K A, Lin J Y and Odom T W 2011 Nanoparticle
SERS substrates with 3D Raman-active volumes Chem. Sci.
 Park W H and Kim Z H 2010 Charge transfer enhancement in the SERS of a single molecule Nano Lett.10 4040–8  Stiles P L, Dieringer J A, Shah N C and Van Duyne R P 2008
Surface-enhanced Raman spectroscopy Annu. Rev. Anal.
 Gwo S, Chen H Y, Lin M H, Sun L and Li X 2016 Nanomanipulation and controlled self-assembly of metal nanoparticles and nanocrystals for plasmonics Chem. Soc.
 Dhawan A, Du Y, Yan F, Gerhold M D, Misra V and Vo-Dinh T 2010 Methodologies for developing surface- enhanced raman scattering(SERS) substrates for detection of chemical and biological molecules IEEE Sens. J.10 608–16
 Tian Z-Q, Ren B and Wu D-Y 2002 Surface-enhanced raman scattering: from noble to transition metals and from rough surfaces to ordered nanostructures Econ. Bot.106 9463–82  Ahmed W, Demirtaş Ö, Öztürk İ M and Bek A 2020
Monolayer assembly of multispiked gold nanoparticles for
surface-enhanced raman spectroscopy-based trace detection of dyes and explosives ACS Appl. Nano Mater.3 6766–73  Staleva H et al 2009 Nanophotonics: plasmonics and metal
nanoparticles Phys. Chem. Chem. Phys.11 5866  Kahraman M, Daggumati P, Kurtulus O, Seker E and
Wachsmann-Hogiu S 2013 Fabrication and characterization of ﬂexible and tunable plasmonic nanostructures Sci. Rep.3 1–9  Schatz G C, Duyne R P V, Zhao J, Dieringer J A and Zhang X
2008 Wavelength-scanned surface-enhanced resonance raman excitation spectroscopy J. Phys. Chem. C112 19302–10
 Schlücker S 2014 Surface-enhanced raman spectroscopy:
concepts and chemical applications Angew. Chemie - Int.
 Kumar G V P 2012 Plasmonic nano-architectures for surface enhanced Raman scattering: a review J. Nanophoton.6 064503  Fleischmann M, Hendra P J and McQuillan A J 1974 Raman
spectra of pyridine adsorbed at a silver electrode Chem.
Phys. Lett.26 163–6
 Albrecht M G and Creighton J A 1977 Anomalously intense raman spectra of pyridine at a silver electrode J. Am. Chem.
 Jeanmaire D L and VAN D R P 1977 Surface Raman spectroelectrochemistry :I. Heterocyclic J. Electroanal.
 Moskovits M 1978 Surface roughness and the enhanced intensity of Raman scattering by molecules adsorbed on metals J. Chem. Phys.69 4159–61
 Kim B, Tripp S L and Wei A 2001 Self-organization of large gold nanoparticle arrays J. Am. Chem. Soc.123 7955–6  Abu Hatab N A, Oran J M and Sepaniak M J 2008 Surface-
enhanced Raman spectroscopy substrates created via electron beam lithography and nanotransfer printing ACS Nano2 377–85
 And C L H and Duyne R P V 2001 Nanosphere lithography: a versatile nanofabrication tool for studies of size-dependent nanoparticle optics J. Phys. Chem. B105 5599–611  Colson P, Henrist C and Cloots R 2013 Nanosphere
lithography: a powerful method for the controlled manufacturing of nanomaterials J. Nanomater.2013 1–19  Zhang X and Van Duyne R P 2005 Optimized silver ﬁlm over
nanosphere surfaces for the biowarfare agent detection based on surface-enhanced Raman spectroscopy Mater. Res. Soc.
Symp. Proc.876 207–12
 Zhang X, Yonzon M A, Stuart D A and Van Duyne R P 2005 Surface-enhanced Raman spectroscopy biosensors:
excitation spectroscopy for optimisation of substrates fabricated by nanosphere lithography IEE Proc.
 Abdelsalam M E, Mahajan S, Bartlett P N, Baumberg J J and Rusell A E 2007 SERS at structured palladium and platinum surfaces J. Am. Chem. Soc.129 7399–406
 Stropp J, Trachta G, Brehm G and Schneider S 2003 A new version of AgFON substrates for high-throughput analytical SERS applications J. Raman Spectrosc.34 26–32
 Lin W C, Liao L S, Chen Y H, Chang H C, Tsai D P and Chiang H P 2011 Size dependence of nanoparticle-SERS enhancement from silverﬁlm over nanosphere (AgFON) substrate Plasmonics6 201–6
 Nardelli M B et al 2008 Corrected 19 december 2008; see last page Science321 388–93
 Xiao G N, Huang W B and Li Z H 2017 Rapid and sensitive detection of malachite green and melamine with silverﬁlm over nanospheres by surface-enhanced Raman scattering Plasmonics12 1169–75
 Lee J, Zhang Q, Park S, Choe A, Fan Z and Ko H 2016 Particle-Film plasmons on periodic silverﬁlm over nanosphere(AgFON): a hybrid plasmonic nanoarchitecture
for surface-enhanced Raman spectroscopy ACS Appl. Mater.
 Flores-Romero E, Rodríguez-Sevilla E and Cheang-Wong J C 2018 Silverﬁlms over silica microspheres (AgFOSM) as SERS substrates Photon. Nanostruct. - Fundam. Appl.28 81–7  Baia L, Baia M, Popp J and Astilean S 2006 Gold ﬁlms
deposited over regular arrays of polystyrene nanospheres as highly effective SERS substrates from visible to NIR J. Phys. Chem. B110 23982–6
 Farcau C, Giloan M, Vinteler E and Astilean S 2012 Understanding plasmon resonances of metal-coated colloidal crystal monolayers Appl. Phys. B106 849–56
 Zhang X, Young M A, Lyandres O and Van Duyne R P 2005 Rapid detection of an anthrax biomarker by surface-enhanced Raman spectroscopy J. Am. Chem. Soc.127 4484–9  Ma K, Yuen J and Shah N 2011 In vivo, transcutaneous
glucose sensing using surface-enhanced spatially offset Raman spectroscopy: multiple rats, improved hypoglycemic accuracy, low incident power, and continuous monitoring for greater than 17 days Anal Chem.83 9146–52  Lyandres O, Shah N C, Yonzon C R, Walsh J T,
Glucksberg M R and Van Duyne R P 2005 Real-time glucose sensing by surface-enhanced Raman spectroscopy in bovine plasma facilitated by a mixed decanethiol/ mercaptohexanol partition layer Anal. Chem.77 6134–9  Himmelhaus M and Takei H 2000 Cap-shaped gold
nanoparticles for an optical biosensor Sensors Actuators B 63 24–30
 Ngo H T, Wang H N, Fales A M and Vo-Dinh T 2013 Label- free DNA biosensor based on SERS molecular sentinel on nanowave chip Anal. Chem.85 6378–83
 Zhu X, Shi L, Liu X, Zi J and Wang Z 2010 A mechanically tunable plasmonic structure composed of a monolayer array of metal-capped colloidal spheres on an elastomeric substrate Nano Res.3 807–12
 Wang J, Zhou F, Duan G, Li Y, Liu G, Su F and Cai W 2014 A controlled Ag–Au bimetallic nanoshelled microsphere array and its improved surface-enhanced Raman scattering effect RSC Adv.4 8758–63
 Greeneltch N G, Blaber M G, Schatz G C and Van Duyne R P 2013 Plasmon-sampled surface-enhanced raman excitation spectroscopy on silver immobilized nanorod assemblies and optimization for near infrared(λex=1064 nm) studies J. Phys. Chem. C117 2554–8
 Ingram W M, Han C, Zhang Q and Zhao Y 2015 Optimization of Ag-Coated polystyrene nanosphere substrates for quantitative surface-enhanced raman spectroscopy analysis J. Phys. Chem. C119 27639–48
 Seyedpour Esmaeilzad N, Demir A K, Hajivandi J,
Ciftpinar H, Turan R, Kurt H and Bek A 2021 Nanosphere concentrated photovoltaics with shape control Adv. Opt.
 Johnson P B and Christy R W 1972 Optical constant of the noble metals Phys. Rev. B6 4370–9
 Le R E C, Blackie E, Meyer M and Etchegoin P G 2007 Surface enhanced Raman scattering enhancement factors: a comprehensive study J. Phys. Chem. C111 13794–803  Kamaliya B, Mote R G, Aslam M and Fu J 2019 Improved
enhancement factor for SERS using broad ion beam induced self-organized gold nanocones MRS Adv.4 697–703  Le Ru E C, Blackie E, Meyer M and Etchegoin P G 2009
Single-molecule surface-enhanced raman spectroscopy of nonresonant molecules J. Am. Chem. Soc.131 14466–72  Le Ru E C and Etchegoin P G 2009 A quick overview of
surface-enhanced Raman spectroscopy Principles of surface-enhanced raman spectroscopy( Amsterdam:
 Postaci S, Yildiz B C, Bek A and Tasgin M E 2018 Silent enhancement of SERS signal without increasing hot spot intensities Nanophotonics7 1687–95